Chemisorption of alkyl phosphate on imogolite nanotubes
As mentioned above, imogolite is a very useful inorganic nanotube. The adsorption and assembly of organic molecules on the imogolite surface is expected to produce interesting results. Imogolite may act as a one-dimensional scaffold for functional molecules. Moreover, the surface energy of imogolite nanotubes can be lowered by the organic layer, and this can greatly improve the dispersibility of imogolite in organic solvents, as well as in various polymer matrices and nanocomposites. The metal–oxygen–phosphorus (M–O–P) interaction plays an important role for surface functionalization of imogolite nanotubes. The strong affinity between octadecylphosphonic acid and the imogolite surface has been reported by our group [32
]. More recently, we developed an approach for anchoring alkyl chains on an imogolite surface from aqueous solution [33
]. The adsorption of molecules on the inorganic surface from aqueous solution is particularly necessary for imogolite, because imogolite nanotubes are dispersible only in water, due to their AlOH surface. For this purpose, a step toward the modification of imogolite nanotubes at the nanotube level with alkyl phosphate from an aqueous solution was achieved by converting the water-insoluble alkyl phosphate into the corresponding water-soluble ammonium salt. The detailed assembly procedure is shown in . The ammonium salt of dodecylphosphate (DDPO4
) was precipitated from a 2-propanol solution of dodecylphosphoric acid (DDPO4
) by the addition of ammonia. The outer surface of imogolite nanotubes is composed of aluminol groups, thus, it can be positively charged and dispersed under acidic conditions by electrostatic repulsion. It should be noted that surface modification of inorganic nanostructures in an aqueous solution is an environmentally friendly method.
Figure 4 Schematic illustration of dodecylphosphate chemisorbing onto the surface of individually dispersed imogolite nanotubes: (a) Dispersion of freeze-dried imogolite powder into weak acidic water by electrostatic repulsion; (b) chemisorption of dodecylphosphate (more ...)
shows the thermogravimetric profiles of the original imogolite, DDPO4-imogolite, and DDPO4H2. The synthetic imogolite loses 30% of its total mass in two steps. The first step is from 300 to 420 K with a weight loss of 13.5%, and the second step is from 420 to 800 K with a weight loss of 16.5%. The first step is attributed to the loss of adsorbed water, while the second one corresponds to the dehydroxylation of imogolite. DDPO4-imogolite has a similar weight-loss profile, although the second step also includes the decomposition of dodecylphosphate. The weight loss in the first step is 8.5%, while in the second step it is 33.5%. DDPO4H2 loses 70% of its initial mass at 800 K, indicating that phosphate groups are left over after the thermal decomposition. Thus, taking the weight loss of imogolite and dodecylphosphate into account, the imogolite content in DDPO4-imogolite is calculated to be 65.6%. Moreover, dodecyl phosphate exhibits an improved thermal stability in DDPO4-imogolite compared with the neat dodecylphosphoric acid. The onset decomposition temperature for DDPO4H2 is 420 K; while for the immobilized dodecyl phosphate the temperature increases to 520 K. This may be because, at the same temperature, the thermal motion of the anchored dodecylphosphate molecules is significantly restricted compared to the unanchored ones.
Thermogravimetric profiles of the original imogolite, DDPO4H2, and DDPO4-imogolite in N2 atmosphere at a heating rate of 10 K min−1.
The interaction between imogolite and DDPO4
is confirmed by IR measurements and X-ray photoelectron spectroscopy (XPS) [33
]. The typical absorption bands of imogolite at 995, 935, and 560 cm−1
still exist, suggesting the retention of the Si–O–Al skeleton in imogolite nanotubes, while the absorption at 995 cm−1
is strengthened by the coexistent absorption of the phosphate groups. The absorption of P=O at 1239 cm−1
and at 1201 cm−1
disappears from the spectrum of DDPO4
-imogolite, presumably due to the condensation between the phosphate groups and the aluminol groups. shows the high-resolution XPS spectra of Al2p
. For the original imogolite, the Al2p
signal is found around 74.3 eV with a symmetric peak; while for DDPO4
-imogolite the Al2p
peak becomes wide and asymmetric, and this can be fitted with two Gaussian curves corresponding to a contribution from peaks at 74.3 eV and 76.3 eV. The second component is ascribed to an increase in the positive charge on Al atoms due to the formation of Al–O–P bonds at the surface of imogolite, while the first indicates the unreacted Al–OH. Thus, it can be concluded that dodecylphosphate attaches to the surface of imogolite through covalent interaction.
Figure 6 High-resolution XPS spectra for Al2p of the original imogolite and DDPO4-imogolite. Adapted with permission from W. Ma et al., Chem. Lett.
40, 159–161 . © 2011, The Chemical Society of Japan.
In order to obtain further insight into the molecular aggregation state of the DDPO4
-imogolite, wide-angle X-ray diffraction (WAXD) measurements were carried out. shows WAXD profiles of the freeze-dried imogolite and DDPO4
-imogolite. Scattering vector q
] is defined as q
= (4π/λ)sinθ, where θ is the scattering angle. The d
-spacing was calculated by d
[nm] = 2π/q
. The WAXD pattern of imogolite consists of a number of diffractions. The diffraction peaks at 2.25, 1.62, 0.93, and 0.67 nm for the freeze-dried imogolite can be assigned to the (100), (110), (001), and (211) planes of the quasi-monoclinic packing of the synthetic imogolite nanotubes [24
]. For DDPO4
-imogolite, the broad diffraction around q
= 13.8 nm−1
is probably due to the disordered grafted alkyl chains. The diffractions at 2.25 and 1.62 nm suggest the presence of imogolite bundles. On the other hand, however, the intensity of the diffractions at 2.25 and 1.62 nm significantly decreased compared with those of the pure imogolite, indicating the exfoliation of the imogolite bundles. Imogolite cylinders may interact through their Al–OH groups, and bundles of imogolite tubes still exist even in weak acidic water. When dodecylphosphate attaches to the surface of these bundles, a one-dimensional core–shell structure forms with imogolite bundles as the core. However, it is expected that only tightly packed bundles can be maintained during the modification process. The modification agent may easily enter the gaps within the loosely packed bundles and adsorb on the surface.
Figure 7 WAXD profiles of (a) original imogolite and (b) DDPO4-imogolite. Adapted with permission from W. Ma et al., Chem. Lett.
40, 159–161 . © 2011, The Chemical Society of Japan.
The individual tubular structure of the dodecylphosphate modified imogolite is directly confirmed by TEM observation. The sample for TEM observation was prepared by placing a drop of the DDPO4-imogolite suspension (toluene as the solvent) on a carbon-coated copper grid and allowing it to dry in air. shows the TEM image of DDPO4-imogolite, in which fiberlike structures with a diameter about 2 nm were observed. This diameter is similar to that of the individual imogolite nanotubes, indicating that these are individual tubes rather than bundles. To the best of our knowledge, this is the first observation of individual imogolite nanotubes with a hydrophobic external surface.
Figure 8 TEM image of DDPO4-imogolite. Reprinted with permission from W. Ma et al., Chem. Lett.
40, 159–161 . © 2011, The Chemical Society of Japan.
The wettability of this dodecylphosphate modified imogolite nanotube was evaluated by measurement of the water contact angle (CA) of the DDPO4-imogolite film. DDPO4-imogolite was dispersed in ethanol at a concentration of 2 mg mL−1, and this dispersion was cast onto a silicon wafer by spin coating. For comparison, an aqueous imogolite solution was also cast onto a silicon wafer by the same procedure. The static contact angle was measured by dropping 1 μL water onto the corresponding surface. As shown in , the static contact angle for the original imogolite cast surface was 22°. In contrast, for the DDPO4-imogolite cast surface, the contact angle increased to 93°. This result indicates that the hydrophilicity of the external surface of imogolite is changed upon absorption of DDPO4, which converts the hydrophilic surface of imogolite nanotubes to a hydrophobic one.
Figure 9 Static-contact-angle images of water droplets on a silicon wafer cast with (a) original imogolite and (b) DDPO4-imogolite. Reprinted with permission from W. Ma et al., Chem. Lett.
40, 159–161 . © 2011, The Chemical Society of (more ...)
Poly(methyl methacrylate) grafted imogolite nanotubes
The above content demonstrated the chemisorption of alkyl phosphonic chains on imogolite surface at the nanotube level from an aqueous solution. However, such low-molecular-weight compounds are insufficient to prevent nanotube aggregation. As a better alternative, the grafting of polymer chains from the nanostructure surface has been developed as a powerful technique for homogeneously dispersing nanostructures [34
]. Several strategies can be used to graft polymers from the inorganic surface, including “grafting to”, “grafting through” and “grafting from” approaches [37
]. In many cases, “grafting from” is preferred, in which the polymer chains are in situ grown from the surface by means of surface-initiated polymerization, and the grafting density is higher compared to the “grafting to” and “grafting through” approaches. The “grafting from” process can be performed with various polymerization techniques, from anionic and cationic to free-radical polymerization [39
]. Free-radical polymerization is preferable to ionic processes on economic grounds, because it is easier to perform and much less sensitive to the presence of water.
Recently, we reported the grafting of poly(methyl methacrylate) (PMMA) on the imogolite surface, in which surface-initiated radical polymerization, called “activators regenerated by electron transfer for atom transfer radical polymerization” (ARGET ATRP), was used [40
]. ARGET ATRP is a newly developed controlled/living radical polymerization technique, and has been attracting more and more research interest due to its convenience, e.g., it can be carried out without strict deoxygenation and only needs ppm levels of catalyst [41
]. presents the preparation procedure of a PMMA grafted imogolite nanotube.
Figure 10 Schematic representation for the preparation of a PMMA grafted imogolite nanotubes. Reprinted with permission from W. Ma et al., Chem. Commun.
47, 5813–5815 . © 2011, The Royal Society of Chemistry.
To realize polymerization of MMA from the surface of imogolite nanotubes, a suitable surface-attachable ATRP initiator is needed. So far, various ATRP initiators that can be fixed on inorganic surfaces have been synthesized by several groups [43
]. Among them, surface-attachable groups have almost exclusively been alkoxy- or chlorosilanes. However, organosilanes are not suitable for the modification of imogolite, because surface modification with organosilanes usually needs dry conditions in order to prevent unfavorable side reactions. Whereas with an AlOH functionalized external surface imogolite is a very hydrophilic material and can be dispersed only in acidic water by electrostatic repulsion [48
]. Moreover, surface bonds between organosilane and the external surface of imogolite have been reported to be labile in a humid atmosphere [49
]. On the other hand, organophosphorous compounds appear complementary to organosilanes, as they show an excellent affinity toward metal oxides [14
]. In addition, they are rather insensitive to nucleophilic substitution and prone to heterocondensation (M–O–P bond formation) as compared to homocondensation (P–O–P). Thus, surface modification with organophosphorous compounds has the advantage of being operable in a wide range of solvents from aprotic to protic, and even in water.
In line with the above discussion, we synthesized an initiator carrying a phosphoric acid group, 8-(2-bromo-2-methylpropanoyloxy) octyl phosphoric acid (BMPOPO4
), which was further converted to a water-soluble ammonium salt [BMPOPO4
]. shows the chemical structure of this initiator molecule. To the best of our knowledge, the closest analogous molecules appear in two papers, in which 11-(2-bromoisobutyrate)-undecyl-1-phosphonic acid and its diethyl ester were synthesized [51
]. However, these two molecules were both designed for application in organic solvents and are not soluble in water. The homogeneous modification of the imogolite surface can be achieved by using a water-soluble initiator carrying a surface-attachable group. In addition, the molecule we designed here seems capable of providing the modified imogolite with adequate hydrophobicity, as it contains a relatively long hydrophobic chain.
Figure 11 Chemical structure of BMPOPO4(NH4)2. Reprinted with permission from W. Ma et al., Polymer
52, 5543–5550 . © 2011, Elsevier B.V.
The ATRP initiator BMPOPO4
was immobilized on the imogolite surface from an aqueous solution at room temperature. The pH is an important parameter in this modification reaction. A low pH value is favorable for the fine dispersion of imogolite in water. However, if the pH is too low, the phosphate group may cause the dissolution of metal oxides. It was reported that PhPO(OH)2
can cause the release of aluminum cations from the alumina surface by cleavage of Al–O–Al bonds at pH 4 [54
]. In this work, the acidity of the initial reaction mixture was controlled and set to be pH 5 in order to avoid a similar dissolution process of imogolite, whose external surface is similar to that of alumina. In our case, a pH 5 acetate buffer was employed. The adsorption of BMPOPO4
onto the imogolite surface was confirmed by FT-IR measurements and XPS analysis. FT-IR spectra show that the Al–O–Si vibrations of imogolite at 992 and 930 cm−1
still exist after modification, indicating that this reaction does not destroy the structure of the imogolite nanotube [40
]. The absorbance bands at 2932 cm−1
(C–H) and 1735 cm−1
(C=O) confirm the adsorption of the ATRP initiator onto the imogolite surface, while the absence of the N–H vibration band at 3130 cm−1
indicates that ammonium counter cations do not adsorb onto imogolite. XPS spectra () provide more information on the interaction between the imogolite surface and the ATRP initiator. In the wide-scan XPS spectra of BMPOPO4
-imogolite, the characteristic peaks of P2p
, and Br3d
were found at around 134.5, 191.8, and 70.0 eV, respectively. In addition, no signal of nitrogen was found, further confirming that the ammonium counter cations do not adsorb onto imogolite. The high-resolution XPS spectra of Al2p
show that the peak position of Al2p
shifts from 74.85 to 74.09 eV (, inset) after modification, which is ascribed to a decrease in the positive charge on Al atoms because of the adsorption of the negatively charged phosphate groups. Thus, the initiator is attached onto the imogolite surface possibly through electrostatic adsorption. In this case, the electron density of the surface aluminum atoms becomes higher compared with the unmodified imogolite, due to the influence of the negatively charged phosphate groups. In contrast, the formation of Al–O–P covalent bonds has been reported to cause an increase in the positive charge on Al atoms, as mentioned above. The difference in bonding manner between DDPO4
on the imogolite surface may be due to the different hydrophobicity of these two molecules. The amount of adsorbed BMPOPO4
was estimated to be 49 wt % by thermogravimetric analysis (TGA) [40
Figure 12 Wide-scan XPS spectra of the original imogolite and BMPOPO4-imogolite (inset, high-resolution XPS spectra of Al2p). Reprinted with permission from W. Ma et al., Polymer
52, 5543–5550 . © 2011, Elsevier B.V.
The subsequent ARGET ATRP was carried out by using ascorbic acid (AA) as the reducing agent and anisole as the solvent. Ascorbic acid is insoluble in anisole, hence, the reduction of the Cu(II) complex takes place at the surface of solid ascorbic acid. The slow reaction rate of this heterogeneous redox process is beneficial for building up a necessary equilibrium between the activator (Cu(I) complex) and deactivator (Cu(II) complex). Polymeric products were isolated by precipitation from methanol. GPC data showed that grafted PMMA with molecular weights of M
n = 26600 and 32700, and corresponding molecular weight distributions of M
n = 1.22 and 1.33 were obtained after a polymerization time of 50 and 90 min, respectively. Hence, grafted PMMA with controllable molecular weight can be achieved by controlling the reaction time.
Bare imogolite cannot be dispersed in any organic solvent, but after modification with BMPOPO4, the resulting modified imogolite can be dispersed in various solvents. Unfortunately, the dispersions are neither homogenous nor stable. However, when PMMA was grafted to the surface of imogolite nanotubes, PMMA-g-imogolite showed good dispersibility in organic solvents, such as THF, chloroform, and toluene. As shown in the homogenous dispersion of PMMA-g-imogolite in THF with a concentration of 10 mg mL−1 was stable for more than two months.
Figure 13 (a) A SFM height image of PMMA grafted imogolite (M
n = 32700, M
n = 1.33). (b) A phase image (insert) and cross-sectional analysis of a PMMA-g-imogolite marked with a circle in (a). (c) Height distribution of the above sample as estimated by SFM. (more ...)
Morphology of PMMA grafted imogolite nanotubes was observed with scanning force microscopy (SFM) in a dynamic force microscopy (DFM) mode employing a sharp diamondlike carbon (DLC) tip with a radius of curvature of 1 nm. shows a height image of one sample with M
n = 32700 and M
w = 1.33. Discrete nanostructures were randomly distributed on the mica surface and no aggregation was observed, indicating excellent dispersibility of PMMA grafted imogolite. The high-resolution phase image and the corresponding cross-sectional analysis in indicates that PMMA grafted imogolite renders a hard middle part and a soft edge. This further confirms the core–shell structure of PMMA-g-imogolite. shows the height distribution of the above PMMA-g-imogolite analyzed from 60 SFM images. The average height value was determined to be 10.6 ± 2.5 nm, although there are still some images having heights of more than 15 nm. If we consider the sample with the smallest height value (6 nm) as containing an individual imogolite nanotube at the core, the ones with larger height values are expected to have nanotube bundles as their rigid cores.
Further evidence on the bundle structures was provided by wide-angle X-ray diffraction (WAXD) measurements. As shown in , the diffraction peaks at q
= 2.8, 4.0, 6.8, and 9.6 nm−1
can be assigned to the (100), (110), (001), and (211) planes of the parallel bundles of the imogolite nanotubes, respectively [24
]. For BMPOPO4
modified imogolite, these four diffraction peaks still exist, suggesting the presence of imogolite bundles. In addition, the peaks at around q
= 2.8 and 4.0 nm−1
become sharper than those of the bare imogolite and, as a result, can easily be distinguished from the overlapped profile, indicating the higher regularity of the bundles compared to that of the bare imogolite. Hence, it is reasonable to conclude that during the modification process only highly ordered imogolite bundles can remain. In addition, the diffraction from (001) plane at ca. q
= 6.8 nm−1
becomes much weaker and broader, suggesting that the bundle size significantly decreased along the (001) plane direction. The above results indicate that small-sized imogolite bundles with high regularity form the rigid core of BMPOPO4
-imogolite during the modification process. After surface-initiated polymerization of MMA, these small-sized imogolite bundles become the cores of PMMA-g
-imogolite, and the diffraction of the (100) plane at around q
= 2.8 nm−1
can still be observed. This result is consistent with the explanation for the SFM observation.
Figure 14 WAXD profiles of (a) quartz-glass capillary background, (b) bare imogolite, (c) BMPOPO4-imogolite, and (d) PMMA-g-imogolite with M
n = 32700 and M
n = 1.33. Reprinted with permission from W. Ma et al., Chem. Commun.
47, 5813–5815 [40 (more ...)
Grafting of functionalized molecules (porphyrins, phtalocyanines, viologens, rhodamine B, etc.) onto metal-oxide surfaces of SiO2
, ITO, WO3
, and ZrO2
can induce the formation of well-defined nanoscopic photoactive molecular arrays of heterosupramolecular assemblies [55
]. Imogolite lacks the intrinsic semiconductivity of the carbon nanotube, but it can be an interesting condensed phase for heterosupramolecular systems due to its high surface area for molecular component adsorption, abundance of empty surface sites for covalent binding of acidic anchoring groups, and high stability under ambient conditions. A more promising approach to render aluminosilicate nanotubes semiconducting is by functionalization with conjugated molecules, such as terthiophene with alkyl spacers consisting of –CH2
– and P=O(OH)2
(). Thiophene oligomers have been extensively studied in recent years due to their excellent optic properties. It has been reported that thiophene oligomers exhibit high quantum yields of photoluminescence, both in solution as well as the solid state, and a broad range of fluorescence frequencies in the entire UV–visible and the near-IR spectrum, through molecular engineering [57
Scheme 1 Synthesis pathway for electron donating (HT3P) and accepting (HT3OP) terthiophene of phosphonic acid derivatives. Reprinted with permission from W. O. Yah et al., Bull. Chem. Soc. Jpn.
84, 893–902 . © 2011, The Chemical Society (more ...)
For preparation of terthiophene/imogolite hybrid materials, imogolite solution was added dropwise to a THF solution of 2-(5’’-hexyl-2,2’:5’,2’’-terthiophen-5-yl)ethylphosphonic acid (HT3P) and stirred overnight at room temperature in the dark. The weight ratio of imogolite to HT3P was 1:1. HT3P/imogolite precipitate was obtained by centrifugation of the suspended solution and rinsing with fresh THF three times to remove weakly or nonchemisorbed HT3P. The precipitate was redispersed in deionized water before being freeze dried. Freeze drying of the precipitate resulted in a cottonlike yellow solid. The same preparation method was used for 2-(5’’-hexyl-2,2’:5’,2’’-terthiophen-5-yl)ethylphosphonic acid 1,1-dioxide (HT3OP) to produce the cottonlike pale brown solid of HT3OP/imogolite hybrid. As a control sample, no precipitate was observed for OH group derivatives (HT3OH and HT3OOH) ().
Figure 15 Schematic illustration of imogolite structure and the preparation of terthiophene/imogolite hybrid materials. Reprinted with permission from W. O. Yah et al., Bull. Chem. Soc. Jpn.
84, 893–902 . © 2011, The Chemical Society of (more ...)
In the FTIR spectrum of HT3P/imogolite hybrid in , the spectrum showed the characteristic absorptions corresponding to the CH2
stretching vibration of HT3P at 2850–2950 cm–1
. The broadness of the peaks in the P–O region between 1200 and 900 cm–1
makes the result difficult to interpret, but the greatly diminished absorption at 2200–2500 cm–1
assigned to the OH stretching of the phosphonic acid groups indicates that the phosphonate headgroup strongly interacted with the imogolite surface [61
]. In addition, the absence of the 1004 cm–1
band, which is assigned to P–O–H groups [62
], was another indication that HT3P molecules were chemisorbed onto the surface of the imogolite nanofiber. The FTIR spectrum of HT3OP/imogolite hybrid as shown in gives a similar result with the disappearance of P–O–H at around 1011 cm–1
suggesting that HT3OP molecules also undergo chemisorptions when in contact with imogolite.
Figure 16 FTIR spectra (a) of HT3P/imogolite hybrid, HT3P, and imogolite, (b) of HT3OP/imogolite hybrid, HT3OP, and imogolite. Reprinted with permission from W. O. Yah et al., Bull. Chem. Soc. Jpn.
84, 893–902 . © 2011, The Chemical Society (more ...)
To investigate the optical properties of terthiophenes on the imogolite surface, a comparison of the UV–vis spectra of terthiophenes (HT3P and HT3OP)/imogolite hybrid between their solutions and solid-state counterparts was made (). Blue-shifting was observed in the spectra of the solvent-cast film for both terthiophene hybrids to a different extent, and with a significantly broadened band. The spectral changes upon solidification from solution arise from two factors: Planarity and intermolecular interaction [64
]. Normally, red-shifting occurs in the solid state when the molecular backbone is more planar compared to the isolated state in solution, due an increase in conjugation length. Thus, the blue-shifting observed in the spectra of thiophene/imogolite films compared to solution indicates that additional an intermolecular interaction was present that plays a role in controlling the solid-state optical properties [65
Figure 17 Normalized solid-state (cast film), imogolite hybrid and solution absorption spectra of (a) HT3P and (b) HT3OP. Reprinted with permission from W. O. Yah et al., Bull. Chem. Soc. Jpn.
84, 893–902 . © 2011, The Chemical Society (more ...)
Fluorescence spectroscopy is a suitable analytical tool for monitoring the intermolecular interactions of terthiophene before and after chemisorption on imogolite. The absorption peak of the HT3P/imogolite hybrid at 322 nm, shifted from that of the HT3P in THF solution (λmax
367 nm), provides additional proof for the formation of an H-type intermolecular interaction of terthiophene on the imogolite surface (). The emission spectra also reveal the impact of intermolecular interaction in the hybrid with a peak at 515 nm that was red-shifted with respect to that of the HT3P solution (λmax
445 nm) [67
]. The formation of H-aggregates of HT3OP on the imogolite surface was also evidenced as the absorption peak shows blue-shifting relative to the HT3OP solution (λmax
360 nm). The emission peak in the fluorescence spectrum of HT3OP/imogolite was red-shifted with respect to that of the HT3OP solution (λmax
455 nm), suggesting the presence of an intermolecular interaction [67
]. In the case of HT3OP/imogolite, however, the peaks are shifted to a lesser extent in the fluorescence spectrum compared to those of the HT3P/imogolite hybrid, due to distortion of the HT3OP backbone by S=O groups, which decrease its planarity and π–π interaction causing weaker H-aggregates of HT3OP on the imogolite.
Figure 18 Fluorescence excitation/emission spectra of (a) HT3P, HT3P/imogolite hybrid and (b) HT3OP, HT3OP/imogolite hybrid. The emission wavelengths monitored for the excitation spectra and the excitation wavelengths used for the emission spectra were as follows: (more ...)
Imogolite has been thought of as an insulator since imogolites consist of wide-bandgap alumina and silica. In fact, due to its unique tubular structure and high aspect ratio, imogolite can be used as an electron-emitting material and water sensor in nanoelectronic devices. The conductivities of the pure imogolite and of the terthiophene/imogolite hybrids were investigated by I–V measurement. By coating the pure imogolite or terthiophene/imogolite onto a silicon wafer and connecting by silver paste at two ends, the conductivity was measured by means of a source meter. The I–V plots, of current on the order of milliamperes versus applied bias voltage in the range from −30 to 30 V, are shown in .
I–V curves of imogolite, HT3P/imogolite, and HT3OP/imogolite hybrid. Reprinted with permission from W. O. Yah et al., Bull. Chem. Soc. Jpn.
84, 893–902 . © 2011, The Chemical Society of Japan.
The averaged electrical conductance calculated from the forward bias region of the pure imogolite I
curve is 5.9 µS. It was speculated that the current flow was due to charge hopping on the hydrated imogolite surface. Oh et al. studied the I
characteristics of imogolite and proposed that bound water molecules contribute to the surface conductivity [69
]. The current flow observed was attributed to the ability of OH groups on the imogolite surface to lose or gain positive charge (a proton) from water molecules resulting in a net change of surface charge. The electrical conductance of HT3OP/imogolite was improved to 60.8 µS, which is one order of magnitude greater than that of pure imogolite. It was observed that HT3OP/imogolite shows non-ohmic characteristics in the I
curve, which signifies a disordered packing of HT3OP on the imogolite surface, in which it behaves like a semiconductor or metal–semiconductor Schottky junction. The HT3OP can act as an electron acceptor when interacting with imogolite, in which the high electron affinity of S=O of HT3OP causes a withdrawal of negative charge from imogolite resulting in the effective motion of positive charges on the imogolite surface. The introduction of HT3OP onto the imogolite surface amplifies the p-type conductivity of imogolite, which resembles the phenomenon of chemical doping of carbon nanotubes with alkaline metals [71
]. On the other hand, the electrical conductance of HT3P/imogolite calculated from the forward bias region is 4.5 µS, which is lower than that before HT3P doping. Here, HT3P acts like an electron donor when interacting with imogolite. The p-type conductivity of imogolite is reduced when the HT3P thiophene ring transfers negative charge to imogolite, which restricts the effective motion of positively charged species on the imogolite surface.
Poly(3-hexyl thiophene)/imogolite nanofiber hybrid
Polythiophenes are one of the well-known families of conductive polymers, and their physicochemical properties, such as their synthesis, electrical and mechanical properties, thermochromism, solvatochromism, and crystal structure [75
], have been extensively studied. Their optical properties, conductivity, and field-effect mobility (FEM) strongly depend on chain conformation and the solid-state-packing mode. For example, well-aligned and highly ordered crystalline polythiophene films will lead to significant improvements in conductivity and FEM; whereas the FEM of the disordered polythiophene film was below the detection level [79
]. Generally, solidification of polythiophene by rapid evaporation of the polymeric solution in good solvent can result in a weak crystalline solid without perceptible morphological structure [81
]. On the other hand, the slow cooling from 70 °C to room temperature of a P3HT solution in a poor solvent, such as xylene or anisole, leads to the formation of a fibrous semicrystalline structure (). Nanofiber formation is always accompanied by a color change from orange to dark red, which is referred to as thermochromism [83
Schematic illustration of reversible formation of P3HT nanofiber.
Recently, a chemiresistive sensor based on a nanofiber hybrid of carbon nanotube/poly(3-hexylthiophene)- and carbon nanotube/hexafluoroiso-propanol-substituted polythiophene systems was reported [84
]. Using a simple solution fabrication process, by dispersing carbon nanotubes in a polythiophene solution followed by spin coating of the solution onto a glass substrate, a highly sensitive and selective chemiresistor was successfully developed. Due to the favorable H-binding of the fluoro-alkyl groups of polythiophene to the phosphate ester, the nanofiber hybrid was reported to be able to detect several numbers of chemical warfare agents, such as dimethyl methylphosphonate (DMMP) and sarin gas [85
]. Nevertheless, large-quantity synthesis of carbon nanotubes involves highly expensive and time-consuming preparation processes. Moreover, it is not practical for certain optical applications that use opaque carbon nanotubes, due to its conjugated π-system. Here, imogolite, the transparent hydrous aluminosilicate nanotube material, with its unique nanostructure was proposed as the inorganic nanotube to be hybridized with P3HT nanofibers. Reinforcement of P3HT nanofibers by imogolite is expected to impart additional mechanical and thermal stability to organic compounds, making the resulted hybrid material more durable under the outer environmental conditions. Therefore, it is crucial to develop a facile synthetic method capable of making uniform and template-free imogolite/P3HT nanofiber hybrids in bulk quantities. Such a synthetic method would be useful for tuning the properties of sensors and photovoltaic or light-emitting devices, which are dependent on well-defined low-dimensional structures. In order to improve compatibility with the P3HT nanofibers, hydrophilic Al–OH groups on the imogolite surface were modified with alkyl phosphonic acid substituted terthiophene (HT3P), as shown in . The molecular aggregation states and molecular orientation of the P3HT chain on imogolite were investigated.
Figure 21 Fabrication and proposed molecular arrangement of P3HT/HT3P-imogolite nanofiber hybrid. Reprinted with permission from W. O. Yah et al., J. Phys.: Conf. Ser.
272, 012021 . © IOP Publishing 2011.
displays the evolution of the absorption spectra of the P3HT solution (a) and the P3HT/HT3P-imogolite nanofiber hybrid (b) cooled from 70 °C to 20 °C. Notably, both spectra exhibit a single peak with λmax
of 450 nm at 70 °C. The spectrum resembles that observed for the P3HT/chloroform system indicating that P3HT was completely dissolved in anisole at the higher temperature. When cooled to room temperature, the band intensity at λmax
= 450 nm decreases in both spectra but is compensated by the appearance of vibronic structure at longer wavelengths (500–650 nm). The isosbectic points observed at 489 nm and 525 nm indicate that P3HT and P3HT/HT3P-imogolite exhibit both isolated coil-like conformation and rodlike conformation in the solution [87
]. The isosbectic point of P3HT/HT3P-imogolite is slightly shifted to a longer wavelength compared to P3HT and was ascribed to a larger amount of the P3HT/HT3P-imogolite aggregate. Upon hybridization, HT3P-imogolite greatly restricts the rotational motion of the P3HT backbone, such that it produces a much longer conjugation length than pure P3HT.
Figure 22 UV–vis absorption spectra of P3HT (a) and P3HT/HT3P-imogolite hybrid (b) in anisole (0.0005%) during cooling. Reprinted with permission from W. O. Yah et al., J. Phys.: Conf. Ser.
272, 012021 . © IOP Publishing 2011.
Dynamic force microscopy (DFM) has proved to be a powerful tool for the direct observation of the aggregation of polymeric nanofibers. By spin coating a dilute solution in anisole, a network of nanofibers more or less entirely covers the silicon substrate. The dimensions of the nanofiber were determined from DFM images; as shown in , P3HT nanofibers have a width and a length on the order of ca. 15 nm and 1 μm, respectively. The thickness, as estimated from the height image of DFM, was on the order of ca. 5 nm. On the other hand, it was observed that the heights of the nanofiber hybrids were 2 to 3 times larger than that of the P3HT nanofiber, indicating the formation of the bundle of the imogolite nanofiber [22
]. Judging from the DFM images, the nanofiber hybrid as shown in exhibited a swollen morphology compared to the pure P3HT nanofiber. It was speculated that the swollen morphology was caused by the intertwining effect of the P3HT nanofiber with the imogolite bundle.
Figure 23 DFM images of (a) P3HT nanofiber and (b) P3HT/HT3P-imogolite nanofiber hybrid. Adapted with permission from W. O. Yah et al., J. Phys.: Conf. Ser.
272, 012021 . © IOP Publishing 2011.
Recent studies on P3HT by grazing-incidence X-ray diffraction revealed the crystallinity and nanostructure in the nanofiber. The structure of P3HT nanofibers is similar to crystalline microdomains in which the P3HT chains pack in lamellar sheets perpendicular to the nanofiber axis. The orientation of the P3HT crystalline phase on the imogolite surface was studied by grazing-incidence wide-angle X-ray diffraction (GIWAXD), as shown in . The out-of-plane GIWAXD pattern revealed only those crystalline plane positions that are in a direction parallel to the x–y axis. Likewise, in the in-plane GIWAXD pattern, only crystalline planes aligned to the z-axis are revealed.
Figure 24 Out-of-plane (a) and in-plane (b) GIWAXD patterns of P3HT/HT3P-imogolite nanofiber hybrid. (c) Schematic illustration of the molecular arrangement of P3HT on imogolite. Reprinted with permission from W. O. Yah et al., J. Phys.: Conf. Ser.
272, (more ...)
In the out-of-plane GIWAXD pattern, the peaks at d = 4 (100) and 7.8 nm (200) were attributed to the ordering of the P3HT hexyl side chains. In other words, the nanofiber height corresponds to the stacking of the hexyl side chains and was parallel to the z-axis of the unit cell. The intensity at (100) was dramatically reduced when the incidence angle, αi = 0.08°, was increased to 0.16°, suggesting that the semicrystalline P3HT mostly resides on the outermost region of the nanofiber hybrid. For the in-plane GIWAXD pattern, one noticeable diffraction peak associated with the (010) diffraction was observed. The diffraction peak corresponds to the π–π* stacking of the P3HT thiophene ring and was parallel to the y-axis, i.e., the nanofiber direction. Again, the (010) peak was diminished when the incidence angle, αi = 0.08°, was increased to 0.16°. These results indicate that P3HT chains reside on the outermost region of nanofiber hybrid along the imogolite axis.